We need your consent to use the individual data so that you can see information about your interests, among other things. Click "OK" to give your consent.
Standard Test Method for Measurement of the Surface Tension of Solid Coatings, Substrates and Pigments using Contact Angle MeasurementsTranslate name
STANDARD published on 1.1.2022
Designation standards: ASTM D7490-13(2022)
Publication date standards: 1.1.2022
The number of pages: 4
Approximate weight : 12 g (0.03 lbs)
Country: American technical standard
Category: Technical standards ASTM
adhesion, contact angles, dispersion and polar components of solid surface tension, solid surface tension, wetting,, ICS Number Code 87.040 (Paints and varnishes)
|Significance and Use|
5.1The method described in this standard is based on the concept that the total free energy at a surface is the sum of contributions from different intermolecular forces, such as dispersion, polar and hydrogen bonding. There are other techniques that employ three components (dispersion, polar and hydrogen bonding). These methods are further complicated by needing three to five test liquids and are not practical for routine testing. This method uses contact angles of two liquids to provide data for the calculation of two components, dispersion, ?sd, and polar, ?sp.
5.2Dispersion and polar component data, along with the total solid surface tension, are useful for explaining or predicting wetting or adhesion, or both, of coatings on pretreatments, substrates and other coatings. Low solid surface tension values often are a sign of contamination and portend potential wetting problems. High polar components may signal polar contamination. There is evidence in the literature that matching of polar components of topcoats and primers gives better adhesion.5.3Solid surface tensions of pigments, particularly the polar components, may be useful in understanding dispersion problems or to provide signals for the composition of dispersants and mill bases. However, comparison of pigments may be difficult if there are differences in the roughness or porosity, or both, of the disks prepared from them.
5.4Although this technique is very useful in characterizing surfaces, evaluating surface active additives and explaining problems, it is not designed to be a quality control or specification test.
1.1This test method describes a procedure for the measurement of contact angles of two liquids, one polar and the other nonpolar, of known surface tension on a substrate, pigment (in the form of a disk), or cured or air dried coating in order to calculate the surface properties (surface tension and its dispersion and polar components) of the solid.
1.2The total solid surface tension range that can be determined using this method is approximately 20 to 60 dyn/cm.
1.3The values stated in CGS units (dyn/cm) are to be regarded as standard. No other units of measurement are included in this standard.
1.4This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.5This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
|2. Referenced Documents|
Do you want to make sure you use only the valid technical standards?
We can offer you a solution which will provide you a monthly overview concerning the updating of standards which you use.
Would you like to know more? Look at this page.
Latest update: 2022-12-04 (Number of items: 2 644 225)
© Copyright 2022 NORMSERVIS s.r.o.